#------------------------------------------------------------------------------
#$Date: 2024-04-05 01:43:12 +0300 (Fri, 05 Apr 2024) $
#$Revision: 290836 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/09/1570955.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1570955
loop_
_publ_author_name
'Chen, Liang'
'Cao, Yili'
'Ma, Rui'
'Cao, Hongmei'
'Chen, Xin'
'Lin, Kun'
'Li, Qiang'
'Deng, Jinxia'
'Liu, Chunyu'
'Wang, Yilin'
'Huang, Ling'
'Xing, Xianran'
_publ_section_title
;
 Regulating luminescence thermal enhancement in negative thermal expansion
 metal-organic frameworks.
;
_journal_issue                   10
_journal_name_full               'Chemical science'
_journal_page_first              3721
_journal_page_last               3729
_journal_paper_doi               10.1039/d3sc06710f
_journal_volume                  15
_journal_year                    2024
_chemical_formula_moiety         'C96 Eu12 N12 O64'
_chemical_formula_sum            'C96 Eu12 N12 O64'
_chemical_formula_weight         4168.60
_chemical_name_systematic        4
_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_atom_sites_solution_primary     direct
_audit_creation_date             2023-12-05
_audit_creation_method
;
Olex2 1.5
(compiled 2023.08.24 svn.re1ec1418 for OlexSys, GUI svn.r6817)
;
_audit_update_record
;
2023-12-05 deposited with the CCDC.	2024-01-30 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   21.6449(8)
_cell_length_b                   21.6449(8)
_cell_length_c                   21.6449(8)
_cell_measurement_reflns_used    1281
_cell_measurement_temperature    250
_cell_measurement_theta_max      29.5660
_cell_measurement_theta_min      2.6490
_cell_volume                     10140.7(6)
_computing_cell_refinement       'CrysAlisPro 1.171.42.86a (Rigaku OD, 2023)'
_computing_data_collection       'CrysAlisPro 1.171.42.86a (Rigaku OD, 2023)'
_computing_data_reduction        'CrysAlisPro 1.171.42.86a (Rigaku OD, 2023)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2019/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXS  (Sheldrick, 2008)'
_diffrn_ambient_temperature      250
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.889
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω    -56.00 -19.00   0.50    6.00    --  -17.65 108.00  83.00   74
  2  ω      4.00  30.00   0.50    6.00    --  -17.65 -99.00 -90.00   52
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy R, DW system, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0150001000
_diffrn_orient_matrix_UB_12      0.0014742000
_diffrn_orient_matrix_UB_13      -0.0290398000
_diffrn_orient_matrix_UB_21      0.0000705000
_diffrn_orient_matrix_UB_22      0.0327787000
_diffrn_orient_matrix_UB_23      0.0015868000
_diffrn_orient_matrix_UB_31      0.0291366000
_diffrn_orient_matrix_UB_32      0.0006640000
_diffrn_orient_matrix_UB_33      -0.0149892000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0460
_diffrn_reflns_av_unetI/netI     0.0397
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.889
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            2863
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.889
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.345
_diffrn_reflns_theta_min         3.121
_diffrn_source                   'Rotating-anode X-ray tube'
_diffrn_source_type              'Rigaku (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    3.712
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.62051
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.86a (Rigaku Oxford Diffraction, 2023)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear light yellow'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    1.365
_exptl_crystal_description       octahedral
_exptl_crystal_F_000             3856
_exptl_crystal_size_max          0.01
_exptl_crystal_size_mid          0.01
_exptl_crystal_size_min          0.01
_refine_diff_density_max         0.961
_refine_diff_density_min         -0.846
_refine_diff_density_rms         0.158
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.037
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     33
_refine_ls_number_reflns         679
_refine_ls_number_restraints     12
_refine_ls_restrained_S_all      1.049
_refine_ls_R_factor_all          0.0575
_refine_ls_R_factor_gt           0.0437
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0791P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1168
_refine_ls_wR_factor_ref         0.1218
_reflns_Friedel_coverage         0.000
_reflns_number_gt                515
_reflns_number_total             679
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3sc06710f2.cif
_cod_data_source_block           Eu-NH2-BDC_250K
_cod_depositor_comments
'Adding full bibliography for 1570952--1570966.cif.'
_cod_original_cell_volume        10140.7(11)
_cod_database_code               1570955
_shelx_shelxl_version_number     2019/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.964
_shelx_estimated_absorpt_t_min   0.964
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(C3) \\sim Ueq, Uanis(N1) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
2. Others
 Fixed Sof: N1(0.125)
;
_smtbx_masks_void_probe_radius   1.0
_smtbx_masks_void_truncation_radius 1.2
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.395
_oxdiff_exptl_absorpt_empirical_full_min 0.839
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x, z'
'-x, -y, z'
'y, -x, z'
'x, -z, y'
'x, -y, -z'
'x, z, -y'
'z, y, -x'
'-x, y, -z'
'-z, y, x'
'z, x, y'
'y, z, x'
'-y, -z, x'
'z, -x, -y'
'-y, z, -x'
'-z, -x, y'
'-z, x, -y'
'y, -z, -x'
'y, x, -z'
'-y, -x, -z'
'-x, z, y'
'-x, -z, -y'
'z, -y, x'
'-z, -y, -x'
'x, y+1/2, z+1/2'
'-y, x+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'y, -x+1/2, z+1/2'
'x, -z+1/2, y+1/2'
'x, -y+1/2, -z+1/2'
'x, z+1/2, -y+1/2'
'z, y+1/2, -x+1/2'
'-x, y+1/2, -z+1/2'
'-z, y+1/2, x+1/2'
'z, x+1/2, y+1/2'
'y, z+1/2, x+1/2'
'-y, -z+1/2, x+1/2'
'z, -x+1/2, -y+1/2'
'-y, z+1/2, -x+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, -z+1/2, -x+1/2'
'y, x+1/2, -z+1/2'
'-y, -x+1/2, -z+1/2'
'-x, z+1/2, y+1/2'
'-x, -z+1/2, -y+1/2'
'z, -y+1/2, x+1/2'
'-z, -y+1/2, -x+1/2'
'x+1/2, y, z+1/2'
'-y+1/2, x, z+1/2'
'-x+1/2, -y, z+1/2'
'y+1/2, -x, z+1/2'
'x+1/2, -z, y+1/2'
'x+1/2, -y, -z+1/2'
'x+1/2, z, -y+1/2'
'z+1/2, y, -x+1/2'
'-x+1/2, y, -z+1/2'
'-z+1/2, y, x+1/2'
'z+1/2, x, y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, -z, x+1/2'
'z+1/2, -x, -y+1/2'
'-y+1/2, z, -x+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, -z, -x+1/2'
'y+1/2, x, -z+1/2'
'-y+1/2, -x, -z+1/2'
'-x+1/2, z, y+1/2'
'-x+1/2, -z, -y+1/2'
'z+1/2, -y, x+1/2'
'-z+1/2, -y, -x+1/2'
'x+1/2, y+1/2, z'
'-y+1/2, x+1/2, z'
'-x+1/2, -y+1/2, z'
'y+1/2, -x+1/2, z'
'x+1/2, -z+1/2, y'
'x+1/2, -y+1/2, -z'
'x+1/2, z+1/2, -y'
'z+1/2, y+1/2, -x'
'-x+1/2, y+1/2, -z'
'-z+1/2, y+1/2, x'
'z+1/2, x+1/2, y'
'y+1/2, z+1/2, x'
'-y+1/2, -z+1/2, x'
'z+1/2, -x+1/2, -y'
'-y+1/2, z+1/2, -x'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, -z+1/2, -x'
'y+1/2, x+1/2, -z'
'-y+1/2, -x+1/2, -z'
'-x+1/2, z+1/2, y'
'-x+1/2, -z+1/2, -y'
'z+1/2, -y+1/2, x'
'-z+1/2, -y+1/2, -x'
'-x, -y, -z'
'y, -x, -z'
'x, y, -z'
'-y, x, -z'
'-x, z, -y'
'-x, y, z'
'-x, -z, y'
'-z, -y, x'
'x, -y, z'
'z, -y, -x'
'-z, -x, -y'
'-y, -z, -x'
'y, z, -x'
'-z, x, y'
'y, -z, x'
'z, x, -y'
'z, -x, y'
'-y, z, x'
'-y, -x, z'
'y, x, z'
'x, -z, -y'
'x, z, y'
'-z, y, -x'
'z, y, x'
'-x, -y+1/2, -z+1/2'
'y, -x+1/2, -z+1/2'
'x, y+1/2, -z+1/2'
'-y, x+1/2, -z+1/2'
'-x, z+1/2, -y+1/2'
'-x, y+1/2, z+1/2'
'-x, -z+1/2, y+1/2'
'-z, -y+1/2, x+1/2'
'x, -y+1/2, z+1/2'
'z, -y+1/2, -x+1/2'
'-z, -x+1/2, -y+1/2'
'-y, -z+1/2, -x+1/2'
'y, z+1/2, -x+1/2'
'-z, x+1/2, y+1/2'
'y, -z+1/2, x+1/2'
'z, x+1/2, -y+1/2'
'z, -x+1/2, y+1/2'
'-y, z+1/2, x+1/2'
'-y, -x+1/2, z+1/2'
'y, x+1/2, z+1/2'
'x, -z+1/2, -y+1/2'
'x, z+1/2, y+1/2'
'-z, y+1/2, -x+1/2'
'z, y+1/2, x+1/2'
'-x+1/2, -y, -z+1/2'
'y+1/2, -x, -z+1/2'
'x+1/2, y, -z+1/2'
'-y+1/2, x, -z+1/2'
'-x+1/2, z, -y+1/2'
'-x+1/2, y, z+1/2'
'-x+1/2, -z, y+1/2'
'-z+1/2, -y, x+1/2'
'x+1/2, -y, z+1/2'
'z+1/2, -y, -x+1/2'
'-z+1/2, -x, -y+1/2'
'-y+1/2, -z, -x+1/2'
'y+1/2, z, -x+1/2'
'-z+1/2, x, y+1/2'
'y+1/2, -z, x+1/2'
'z+1/2, x, -y+1/2'
'z+1/2, -x, y+1/2'
'-y+1/2, z, x+1/2'
'-y+1/2, -x, z+1/2'
'y+1/2, x, z+1/2'
'x+1/2, -z, -y+1/2'
'x+1/2, z, y+1/2'
'-z+1/2, y, -x+1/2'
'z+1/2, y, x+1/2'
'-x+1/2, -y+1/2, -z'
'y+1/2, -x+1/2, -z'
'x+1/2, y+1/2, -z'
'-y+1/2, x+1/2, -z'
'-x+1/2, z+1/2, -y'
'-x+1/2, y+1/2, z'
'-x+1/2, -z+1/2, y'
'-z+1/2, -y+1/2, x'
'x+1/2, -y+1/2, z'
'z+1/2, -y+1/2, -x'
'-z+1/2, -x+1/2, -y'
'-y+1/2, -z+1/2, -x'
'y+1/2, z+1/2, -x'
'-z+1/2, x+1/2, y'
'y+1/2, -z+1/2, x'
'z+1/2, x+1/2, -y'
'z+1/2, -x+1/2, y'
'-y+1/2, z+1/2, x'
'-y+1/2, -x+1/2, z'
'y+1/2, x+1/2, z'
'x+1/2, -z+1/2, -y'
'x+1/2, z+1/2, y'
'-z+1/2, y+1/2, -x'
'z+1/2, y+1/2, x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.000000 0.000000 0.12979(3) 0.0266(3) Uani 1 8 d S T P . .
O1 O 0.05934(19) -0.05934(19) 0.05934(19) 0.0186(16) Uani 1 6 d S T P . .
O2 O 0.000000 -0.0983(3) 0.1767(3) 0.069(2) Uani 1 2 d S T P . .
C1 C 0.000000 -0.1546(6) 0.1546(6) 0.086(6) Uani 1 4 d S T P . .
C2 C 0.000000 -0.2034(6) 0.2034(6) 0.125(9) Uani 1 4 d S T P . .
C3 C 0.000000 -0.1822(8) 0.2682(8) 0.142(6) Uani 1 2 d S TU P . .
N1 N 0.000000 -0.1207(16) 0.291(2) 0.081(12) Uani 0.25 2 d S TU P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Eu1 Eu1 Eu1 60.0 101 8 ?
Eu1 Eu1 Eu1 90.0 104 8 ?
Eu1 Eu1 Eu1 60.0 5 8 ?
Eu1 Eu1 Eu1 90.0 5 101 ?
Eu1 Eu1 Eu1 60.0 104 101 ?
Eu1 Eu1 Eu1 60.0 5 104 ?
O1 Eu1 Eu1 33.11(7) . 5 ?
O1 Eu1 Eu1 33.12(7) 2 8 ?
O1 Eu1 Eu1 33.12(7) 2 101 ?
O1 Eu1 Eu1 33.11(7) 4 5 ?
O1 Eu1 Eu1 85.89(14) 4 101 ?
O1 Eu1 Eu1 85.89(14) 3 5 ?
O1 Eu1 Eu1 85.89(14) 4 8 ?
O1 Eu1 Eu1 85.89(14) 2 5 ?
O1 Eu1 Eu1 85.89(14) . 101 ?
O1 Eu1 Eu1 85.89(14) . 104 ?
O1 Eu1 Eu1 85.89(14) 3 8 ?
O1 Eu1 Eu1 33.11(7) 4 104 ?
O1 Eu1 Eu1 33.11(7) . 8 ?
O1 Eu1 Eu1 33.11(7) 3 104 ?
O1 Eu1 Eu1 85.89(14) 2 104 ?
O1 Eu1 Eu1 33.12(7) 3 101 ?
O1 Eu1 O1 65.59(18) 4 3 ?
O1 Eu1 O1 65.59(18) . 4 ?
O1 Eu1 O1 100.0(3) . 3 ?
O1 Eu1 O1 65.59(18) . 2 ?
O1 Eu1 O1 65.59(18) 3 2 ?
O1 Eu1 O1 100.0(3) 4 2 ?
O2 Eu1 Eu1 107.71(12) 4 5 ?
O2 Eu1 Eu1 160.49(19) 2 104 ?
O2 Eu1 Eu1 107.71(12) 2 5 ?
O2 Eu1 Eu1 70.48(19) . 5 ?
O2 Eu1 Eu1 160.48(19) . 101 ?
O2 Eu1 Eu1 107.71(12) 3 104 ?
O2 Eu1 Eu1 107.71(12) . 8 ?
O2 Eu1 Eu1 70.48(19) 3 101 ?
O2 Eu1 Eu1 70.48(19) 4 104 ?
O2 Eu1 Eu1 107.71(12) 3 8 ?
O2 Eu1 Eu1 160.49(19) 3 5 ?
O2 Eu1 Eu1 70.48(19) 2 8 ?
O2 Eu1 Eu1 160.49(19) 4 8 ?
O2 Eu1 Eu1 107.71(12) 2 101 ?
O2 Eu1 Eu1 107.71(12) 4 101 ?
O2 Eu1 Eu1 107.71(12) . 104 ?
O2 Eu1 O1 77.7(2) 3 2 ?
O2 Eu1 O1 139.95(10) 3 4 ?
O2 Eu1 O1 77.7(2) 3 3 ?
O2 Eu1 O1 77.7(2) 2 2 ?
O2 Eu1 O1 77.7(2) 4 4 ?
O2 Eu1 O1 139.95(10) 4 2 ?
O2 Eu1 O1 139.95(10) . 3 ?
O2 Eu1 O1 139.95(10) . 2 ?
O2 Eu1 O1 139.95(10) 2 4 ?
O2 Eu1 O1 139.95(10) 3 . ?
O2 Eu1 O1 77.7(2) . 4 ?
O2 Eu1 O1 77.7(2) 2 . ?
O2 Eu1 O1 77.7(2) 4 3 ?
O2 Eu1 O1 139.95(10) 4 . ?
O2 Eu1 O1 77.7(2) . . ?
O2 Eu1 O1 139.95(10) 2 3 ?
O2 Eu1 O2 79.33(15) 4 . ?
O2 Eu1 O2 79.33(15) 3 2 ?
O2 Eu1 O2 79.33(15) 2 . ?
O2 Eu1 O2 129.0(4) 2 4 ?
O2 Eu1 O2 129.0(4) 3 . ?
O2 Eu1 O2 79.33(15) 3 4 ?
Eu1 O1 Eu1 113.77(13) . 8 ?
Eu1 O1 Eu1 113.77(13) . 5 ?
Eu1 O1 Eu1 113.77(13) 5 8 ?
C1 O2 Eu1 133.1(9) . . ?
O2 C1 O2 132.9(15) . 117 ?
O2 C1 C2 113.5(8) 117 . ?
O2 C1 C2 113.5(8) . . ?
C3 C2 C1 116.9(10) 117 . ?
C3 C2 C1 116.9(10) . . ?
C3 C2 C3 126(2) . 117 ?
C2 C3 C3 116.9(10) . 45_545 ?
N1 C3 C2 128(2) . . ?
N1 C3 C3 115.1(19) . 45_545 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Eu1 Eu1 3.9729(10) 8 ?
Eu1 Eu1 3.9729(10) 5 ?
Eu1 Eu1 3.9729(10) 104 ?
Eu1 Eu1 3.9729(10) 101 ?
Eu1 O1 2.3716(19) 3 ?
Eu1 O1 2.3716(19) . ?
Eu1 O1 2.3716(19) 2 ?
Eu1 O1 2.3716(19) 4 ?
Eu1 O2 2.358(6) 3 ?
Eu1 O2 2.358(6) 4 ?
Eu1 O2 2.358(6) . ?
Eu1 O2 2.358(6) 2 ?
O2 C1 1.308(9) . ?
C1 C2 1.49(2) . ?
C2 C3 1.477(19) . ?
C2 C3 1.477(19) 117 ?
C3 C3 1.52(3) 45_545 ?
C3 N1 1.42(4) . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Eu1 O2 C1 O2 0.000(0) . . . 117 ?
Eu1 O2 C1 C2 180.000(0) . . . . ?
O2 C1 C2 C3 0.000(0) 117 . . 117 ?
O2 C1 C2 C3 180.000(0) 117 . . . ?
O2 C1 C2 C3 0.000(0) . . . . ?
O2 C1 C2 C3 180.000(0) . . . 117 ?
C1 C2 C3 C3 180.000(0) . . . 45_545 ?
C1 C2 C3 N1 0.000(2) . . . . ?
C3 C2 C3 C3 0.0 117 . . 45_545 ?
C3 C2 C3 N1 180.000(1) 117 . . . ?
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 -0.649 -0.431 -0.777 5159.9 1128.9 ?
